4.2.4 Electrochemical behavior
The electrochemical behavior of the interlayer was tested building symmetric Li|LPS|Li cells with and without interlayer between the electrolyte and the alkaline metal, and performing long–term stability tests, by plating and stripping lithium at the electrode|electrolyte interface. Later on, the electrochemical behavior of the interlayer was tested in full–cells with NCM as a cathode material and a lithium metal anode.
In contrast, Figure 38 shows the plating and stripping data of a symmetric Li|LPS|Li cell with P3N5 on both sides of the compressed electrolyte powder. To ensure to get a dense covering layer, 17 nm of P3N5 were deposited on either side of the electrolyte. It needs to be pointed out that a sacrificial layer according to the definition of this work may need to be thinner to protect the battery without inhibiting the transport properties but the surface of pressed LPS powder requires a thicker surface layer.
As can be seen, the cell with interlayer can be cycled with the same settings as the cell without interlayer for over 2000 hours. The potential increases over time, again indicating an increasing cell resistance but the absolute increase of the potential is around 17 mV; as much Figure 37: Lithium plating and stripping of a Li|Li3PS4|Li cell without interlayer at room temperature. For the experiment 100 µA/cm2 were applied for 2 h in each direction. During each step, an 870 nm thick layer of lithium was plated and removed. The experiment could be performed for more than 2000 h. Close–ups of the beginning and the end of the measurement show that the overpotential increases over time and that the plating/stripping is less uniform after 2000 h.
The edges of each step are not perfectly horizontal due to the OCV step in between.
as for the sample without interlayer. The shape of the curve also shows less fluctuations of the overpotential during each plating/stripping step suggesting that a more homogeneous lithium plating and stripping takes place. It is assumed that applying a homogeneous surface layer leads to a more homogenous potential distribution at the interface and cycling behavior because impurities of the LPS powder (e.g. reaction products with atmosphere and carbon impurities that are present up to a certain amount no matter how clean the glovebox atmosphere is), are circumvented and do not hinder the charge transfer anymore.
With an initial value of 50 mV, this cell has a higher overpotential than the cell without interlayer and it increases up to 66 mV after 2000 h. The additional overpotential results from the P3N5 layer between the electrolyte and the lithium electrode. A part of the P3N5
layer is converted into Li3N and Li3P, but as the reaction products limit the electron diffusion Figure 38: Lithium plating and stripping of a Li|P3N5|Li3PS4|P3N5|Li cell with a 17 nm thick interlayer at room temperature. For the experiment 100 µA/cm² were applied for 2 h in each direction. During each step, an 870 nm thick layer of lithium was plated and removed. Thickness of the interlayer: 17 nm. The overpotential is higher than in a cell without interlayer and also increases over time. After 2000 h, plating/stripping is still homogeneous. The edges of each step are not perfectly horizontal due to the OCV step in between.
through the interface, the conversion ceases, and the SEI growth is limited. A part of the P3N5 layer remains unreacted at the interface, inhibiting the charge transfer and increasing the cell resistance. Plating/stripping experiments were also performed at 60 °C (Figure 39).
As can be seen, the initial potential of the sample without interlayer at 60 °C is only 10 mV.
Due to the increased temperature, the cell resistance and overpotential are much lower than at room temperature. The potential remains almost constant for around 120 hours. Then it starts to increase to more than 25 mV, before the cell is short circuited after around 900 hours. This increase of the potential slows down between 250 and 800 hours leading to a parabolic change over time. When in accordance with the observations of the SEI growth on „LiPON“ the interphase shows a parabolic growth, the resistance should show the same behavior. It can therefore be suggested that the increased overpotential is caused by a decomposition of the electrolyte. Taking a closer look at the data, it can be seen that at the beginning the potential at which lithium plating and stripping happens, remains virtually constant during each 2 h step. In comparison it can be seen that after 800 hours, the potential slightly increases during each step.
Figure 39: Lithium plating and stripping of a Li|Li3PS4|Li cell without interlayer at 60 °C.
For the experiment 100 µA/cm² were applied for 2 h in each direction. During each step, an 870 nm thick layer of lithium was plated and removed.
This behavior can be due to different phenomena. It can be caused by a contact loss between lithium and the electrolyte during lithium dissolution, resulting in a smaller interface area and a less homogeneous plating/stripping behavior. It may also be caused by the diffusion of lithium ions through a growing reaction layer.
In comparison, Figure 40 shows data of the best running cell with an interlayer at 60 °C.
The initial overpotential is at 10 mV but after a few plating/stripping steps increases to 14 mV, higher than for the sample without interlayer. The steep increase after a few hours was caused by a breakdown of the power supply overnight and it is unclear what happened.
Aside from that, the observed homogeneous increase of the potential during plating/stripping with constant current is smaller than for the sample without interlayer. The increase of the potential slows down after around 200 hours but continues across the entire duration of the measurement.
Figure 40: Lithium plating and stripping of a Li|P3N5|Li3PS4|P3N5|Li cell with interlayer at 60 °C. For the experiment 100 µA/cm² were applied for 2 h in each direction.
During each step, an 870 nm thick layer of lithium was plated and removed.
Thickness of the protective layer: 17 nm. The results are from the best running cell.
Again, a parabolic increase can be seen but it is almost the same as for the sample without interlayer. Although the resistance increases from cycle to cycle, the potential during each plating and stripping step remains almost constant, indicating that the process is more homogenous than at the unmodified interface.
To determine the influence of the film thickness of the interlayer on the cell performance, the deposition time of P3N5 was decreased to 15 min, reducing the film thickness to ~ 8 nm.
Figure 41 shows a comparison of the plating and stripping data of two samples with P3N5
layer (i.e. the sample from Figure 40 and one with a thinner interlayer) with different film thicknesses at 60 °C and Figure 42 a comparison between a sample without interlayer and the one with an 8 nm thick interlayer.
As can be seen, the overpotential is reduced by 5 mV when the film thickness is halved, indicating that also the cell resistance is decreased. Assuming that 17 nm of P3N5 are too thick to fully react, this observation is reasonable. Still, lithium plating and stripping increases the potential and therefore the cell resistance over time. In the beginning, this increase seems to be slower than in cells with a thicker interlayer, indicating a better protection of the cell or a better plating/stripping behavior. An interlayer of P3N5 with 8 nm thickness may still be thicker than the optimal calculated thickness of the natural passivating material „LiPON“
but it can be expected that the rough inhomogeneous surface of the pressed LPS powder leads to a less conformal deposition than on a smooth thin–film and requires a thicker interlayer.
The sample using 8 nm of P3N5 as interlayer has as high an initial overpotential as the sample without interlayer (Figure 42). Therefore, it be can assumed that the formation of the interphase was prior to the start of the first measurement and must have been finished during the temperature stabilization at 60 °C. Whereas the sample without interlayer does not show an increase of the overpotential and resistance during the first 150 h but increases afterward, the overpotential of the sample with P3N5 layer increases continuously. Compared to the sample without interlayer, this increase is not parabolic but linear and smaller than for the sample without interlayer. A parabolic increase is due to the interphase formation. The absence of a parabolic increase can be explained by two different effects:
a) The electrolyte is protected from decomposition. When no decomposition is caused, the increase of the resistance can be attributed to regular mechanical degradation
mechanisms of the cell during plating/stripping, e.g. volume changes of the electrode, changes of the interface area, and the creation of cracks and pores and relaxation of the electrolyte thickness. In this case the interlayer effectively negates the thermodynamic driving force for the decomposition and thermodynamically stabilizes the lithium|electrolyte contact.
b) The decomposition of the electrolyte is slowed down drastically. If the interlayer does not cover the entire electrolyte surface, a decomposition in contact with lithium metal may still take place but it is so slow that it is superimposed by the regular mechanical degradation.
Figure 41: Comparison of two samples with two different interlayer thicknesses.
Plating/stripping experiments at 60 °C. For the experiment 100 µA/cm² were applied for 2 h in each direction
The 8 nm thick interlayer is still more than twice as thick as the optimal layer thickness that was determined from examinations on „LiPON“. A thinner layer may also protect the electrolyte from decomposition without leading to an increased cell resistance. However, applying a homogeneous interlayer with a thickness smaller than 8 nm on a rough electrolyte surface by IBS is on one hand technically challenging. On the other hand, films with a thickness < 5 nm may lead to problems. In a thickness range of less than a few nanometers, the interlayers may lose their protective effect because electrons may be able to tunnel through the protective layer. In ASSBs, a distinction between failure due to an inhomogeneous interlayer or tunneling through the interlayer is currently not possible.
Figure 42: Comparison of a symmetric cell with and without interlayer. Plating/stripping experiments at 60 °C. For the experiment 100 µA/cm² were applied for 2 h in each direction.